Production, Processing and Assembly of Carbon Nanotubes
by Huaizhi Geng
A dissertation submitted to the faculty of the University of North Carolina at Chapel Hill in partial fulfillment of the requirement for the degree of Doctor of Philosophy in the Curriculum in Applied and Materials Sciences.
Chapel Hill 2006
Huaizhi Geng: Production, Processing and Assembly of Carbon Nanotubes (Under the direction of Professor Otto Zhou)
This dissertation reports the development of a method to achieve continuous production of carbon nanotubes. The as produced carbon nanotubes were purified and further processed to tune their properties. Then dielectrophoresis as a versatile technique was used to manipulate and assemble carbon nanotubes into functional structures.
In the processing part, purified carbon nanotubes are treated with strong acid then annealed at different temperatures. Combined TEM and NMR studies show that tips of SWNTs in bulk quantities can be uniformly opened by oxidation and closed by vacuum annealing at a surprisingly low temperature. The results provide a guideline on how the SWNTs should be processed for potential energy storage applications.
First of all, I would like to thank Dr. Otto Zhou, for being a great teacher and advisor, for constant support and encouragements on my study and research. It is him who introduced me to the field and whose enthusiasm has been a daily source of inspiration. It is also his continuous encouragement, great consideration and patience that make this work possible.
It has been a privilege to work with so many talented people in Dr. Zhou’s research group. I am grateful to several formal and current group members. They are, Dr. B. Gao, Dr. L. Fleming, Dr. H. Shimoda, Dr. J. Zhang, Mr. Q. Qiu , Dr. S. Oh., Ms. R. Rajaram, Ms. X. Calderon and Mr. D. Bordelon.
TABLE OF CONTENTSChapter1 Introduction………..…………...1
1.1 Structure and properties of CNTs………..…………..1
1.1.1 Structure of CNTs………..………...1
1.1.2 Properties of CNTs……….………..4
1.2 Applications of CNTs………….……….………6
1.2.1 Nanoprobes and Sensors………...…….…...7
1.2.2 Field Emitters………..…..9
1.2.3 Other Applications……….….12
1.3 Conclusions and dissertation overview……….…….13
Chapter 2 Synthesis of carbon nanotubes ……….….19
2.2 Summary of currently used synthesis methods……….……19
2.2.1 Arc Discharge……….20
2.2.2 Laser Ablation……….…...21
2.2.3 Chemical Vapor Deposition……….…..24
2.3 The method of Laser-CVD………...….26
2.3.2 Experiment and Results……….27
Chapter 3 Processing of Carbon Nanotubes…….………...………...36
3.2 Purification and Cutting of carbon nanotubes..……….……....37
3.2.1 Purification of carbon nanotubes…………..………..37
3.2.2 Cutting of carbon nanotubes….………..40
3.2.3 Properties of acid treated carbon nanotubes……….……..44
3.3 Regraphitization of carbon nanotube by high temperature annealing…….……..47
3.3.1 HRTEM analysis ………...…….48
3.3.2 Gas absorption experiment and Results.…..……….………..49
Chapter 4 Manipulation and assembly of CNTs by Dielectrophoresis………...55
4.2.1 Dielectrophoretic Force………..56
4.2.2 Torque and Alignment ………...59
4.3 Experimental Setup………62
4.4 Assembly of CNT structures ……….63
4.4.2 Assembly of CNT structures according to field configuration……….68
4.5 A systematic Study on the effects of parameters….………70
4.5.1 Frequency of AC electrical field………...70
4.5.2 Ionic conductivity of suspending medium ……….……..72
4.5.3 Viscosity of suspending medium……….….73
4.5.4 Concentration of the suspention………74
4.6 CNT fibrils fabricated by dielectrophoresis ………..…..75
4.6.1 Fabrications of CNT fibrils………..……….75
4.6.2 Applications of CNT fibrils……….…….77
Chapter 5 Automation and Optimization of the Fabrication of CNT fibrils……...82
5.2 Problems of the Original Experimental Setups and Solutions ………...84
5.3 Automation of the Process……….………..87
5.3.1 Experimental setup………87
5.3.2 Change in capacitance of the system……….89
5.3.3 Labview Program………...91
5.4 Parameter study using the automated experimental setup………...93
5.4.1 Effects of Waiting time ………...………...94
5.4.2 Effects of Voltage………...96
Chapter 1 Introduction
1.1 Structure and Properties of Carbon nanotubes (CNT)
The extraordinary mechanical properties, unique electrical properties, chemical and thermal stability and especially the nano-metric sizes and tubular shapes of carbon nanotubes (CNTs) have stimulated extensive research activities across the world since their discovery by Sumio Iijima of the NEC Corporation in 1991.  The early researches were focused on production and characterization. While more and more intriguing properties were found about CNTs and relatively efficient synthesis methods for producing CNTs with acceptable qualities were developed, investigations focused on application development have increased in numbers.
1.1.1 Structure of CNTs
wall nanotube (SWNT), one atom in wall thickness and tens of atoms around the circumference (typical diameter ~ 1.4 nm). (Figure 1.1 a) The primary products of the synthesis of SWNTs are aggregates of individual tubes forming structure akin to ropes of fibers, which are called SWNT bundles. Figure 1.1 b shows the cross section a SWNT bundle. Multiwall nanotubes (MWNT) are a collection of several concentric graphene tubules that are interconnected by van der Waals force, and their total diameter ranges from 5 nm to 50 nm. (Figure 1.1 c)
Figure 1.1 High resolution transmission electron microscope pictures of (a) An isolated SWNT  (b) Cross section of SWNT bundles. SWNTs produced by laser ablation and arc discharge bundles up because of van der Waals attration. The cross section forms a triangular lattice structure. The diameter of a bundle is between 10 and 50 nm, corresponding to 30-500 tubes per bundle . (a) MWNT, the inner core can be as small as 0.4 nm .
When the graphene sheet is ‘rolled up’ in different angle to form a nanotube, three types of single walled nanotubes are possible. They are called armchair, zigzag and chiral nanotubes respectively. In Figure1.2, the so-called chiral vector of the nanotube, Ch, is defined by Ch =
and m are integers. Another important parameter is the chiral angle, which is the angle between Ch and â1. When the graphene sheet is rolled up to form the cylindrical part of the CNT, the ends of the chiral vector meet each other. The chiral vector thus forms the circumference of the CNT’s circular cross-section, and different values of n and m lead to different CNT structures Armchair nanotubes are formed when n = m and the chiral angle is 30° (see Figure 1.2 (a)) Zigzag nanotubes are formed when either n or m are zero and the chiral angle is 0° (Figure 1.2 (b)). All other nanotubes, with chiral angles intermediate between 0° and 30° are known as chiral nanotubes (Figure 1.2 (c)). In figure 1.3 (a) shows an armchair SWNT, (b) shows a zigzag SWNT and (c) shows a chiral SWNT.
Figure 1.2 Structure of a SWNT related with its chiral vector. (a)A chiral vector Ch = n a1 + m a2 is defined on the honeycomb lattice of carbon atoms by unit vector a1 and a2 and the chiral angle θ with respect to the zigzag axis , (b) A high resolution scanning tunneling
microscopy (STM) image showing the lattice structure of a chiral SWNT. The helical structure is clearly revealed .
Figure 1.3 Different types of SWNT, (a) an armchair SWNT; (b) a zigzag SWNT; (c) a chiral SWNT 
1.1.2 Properties of CNTs
The unique structures of CNTs provide them with many unique properties that attracted tremendous amounts of research and development efforts. The findings have significantly extended our understanding of the fundamental science at the nanometer scale and created the opportunities for future technologies.
From the fundamental physics point of view, SWNTs provide a nearly perfect model system for one-dimensional conductors. Relatively early in the research of nanotubes, Thess et al. calculated the resistivity of ropes of metallic SWNTs to be in the order of 10-4 Ω-cm at 300 K.  Which would indicate that the ropes were the most highly conductive carbon fibers known, even factoring in their error in measurement. It is also reported that  the stable current density of one arc-produced MWNT was able to reach greater than 107 A/cm2. Later, Phaedon Avouris  suggested that stable current densities of MWNTs could be pushed as high as 1013 A/cm2. Furthermore, electronic transport in metallic SWNTs and MWNTs occurs ballistically (i.e., without scattering) over long tube lengths, enabling them to carry high currents with essentially no heating. [11-14]
Research results suggested an unusually high value thermal conductivity of 6600 W/mK, for an isolated (10, 10) nanotube at room temperature, comparable to the thermal conductivity of a
hypothetical isolated graphene monolayer or diamond. [15,16]
Table 1.1 Mechanical properties of Nanotubes  Young’s Modulus
(GPa) Tensile Strength (GPa) Density (g/cm3)
MWNT 1200 ~150 2.6
SWNT 1054 75 1.3
SWNT bundle 563 ~150 1.3
Graphite (in plane) 350 2.5 2.6
Steel 208 0.4 7.8
The porous structure of SWNT bundles and unique electrochemical properties of CNTs also give promising properties as energy storage materials. [24-30]
1.2 Applications of CNTs
7 1.2.1 Nanoprobes and Sensors
Scanning probe microscopy (SPM) has become an essential scientific research tool, particularly in the field of nanoscale science and technology. Because of its versatility, SPM has become one of the techniques for the investigation of single molecule phenomena in areas of scientific research from molecular biology to nanoscale fabrication. SPM is also playing a more and more important role in surface characterization for industrial applications. This is particularly important in semiconductor industries when devices approach sizes below 100nm. Some examples for industrial applications are: magnetic force microscopy (MFM) for characterization of magnetic domains in the data storage industry and general surface roughness characterization of ultra thin films. 
At the heart of SPM is the interaction between the tip of the scanning probe and a sample surface. The geometry and material properties of the tip on the scanning probe ultimately determine the performance and resolution of the instrument as it is show in figure 1.4.
As described in the property section, CNTs with extremely small sizes, high conductivity, high mechanical strength and flexibility, are ideal starting materials for fabrication of Nanoprobes. One could think of such probes as being used in a variety of applications, such as high-resolution imaging, nano-lithography, nanoelectrodes, drug delivery, sensors and field emitters. The possibility of nanotubes-based field emission will be discussed in the next section. The advantage of CNT probe is its slenderness and the possibility to image features with high aspect ratios, which are almost impossible to probe using the larger, blunter etched silicon or metal tips. MWNTs and SWNT bundles are conducting and can also be used as STM probes. Biological molecules, such as DNA can also be imaged with higher resolution using CNT probes, compared to conventional STM probes. In addition, due to the high elasticity of the CNTs, the probes do no suffer from crashes on contact with the sample surfaces. Any impact will cause buckling of the nanotubes, which generally is reversible on retraction of the tip from the surface. Also because CNTs have much higher resistance to abrasion, CNT probes have much longer life times compared with silicon probes. [33-36]
In addition to the use of CNT probes for high-resolution imaging, it is also possible to use CNTs as active tools for surface manipulation. It has been shown that CNT AFM probes being used in nano-lithography. Ten nanometer lines have been written on oxidized silicon substrates using CNT probe. [37,38]
used to perform local chemistry, to measure binding forces between protein-ligand pairs and for imaging chemically patterned substrates. [39-40]
1.2.2 Field Emitters
Electron sources are key components of many modern devices and play a central role in information display. Presently, the most widely used electron source is the bulky thermionic cathode, where a metal filament is heated to 1000-3000°C such that a portion of the electron population has sufficient kinetic energy to overcome the work function of the metal (a few electron volts) to be emitted to vacuum level . Field emission is an alternative mechanism of extracting electrons. It is a quantum mechanical phenomenon in which electrons near the Fermi level escape from a solid surface into vacuum by tunneling through a thinned energy barrier under the influence of an external electric field . In contrast to the commonly used thermionic emission based on a hot filament, field emission occurs at room temperature as an instantaneous response to the applied electric field. Because of several attractive characteristics, including no requirement of heating (therefore, no cooling of the system), fast response to electric field variation, resistance to temperature fluctuation and radiation, and an exponential current-voltage relationship, field emission is a preferred electron emission mechanism for many applications such as flat panel displays, portable X-ray tubes, compact microwave amplifier, and high resolution electron microscopy .
Field emission is also called Fowler-Nordheim tunneling. Fowler-Nordheim equation (I = aV2 exp(-bφ3/2/βV), where I, V, φ, β are emission current density, applied voltage, work
phenomena.  According to the equation, field emission current density depends on the applied voltages, the emitter’s work function and the field enhance factor, which totally depends on the geometry of the emitter. The work function is an intrinsic property of the material that can be lowered by engineering only to a certain degree. However the field enhance factor, which is the slope of the F-N plot, can be tremendously increased by tailoring the geometry of the emitter.
Figure 1.5 Compressed equipotential lines near the sharp protrusion of a metal surface (unit of x and y axis: nm, equipotential spacing: 10V) .
abilities to carry on high current density for extended period of time without building up too much heat, which will cause degradations of the emitters. .
Field emission experiments carried out on individual nanotubes also revealed the excellent emission stability at high current. A single multiwall nanotube emitter was capable of emitting 2 µA current for more than 100 hours , and catastrophic failure did not occur until the current reached as high as 0.2 mA. Single wall nanotubes generally have a smaller diameter and higher degree of structural perfection than multiwall nanotubes, hence a capability for achieving higher current densities and a longer lifetime . The current-voltage characteristics of an individual clean single wall nanotube showed no evidence of current saturation for emission currents reaching 2 µA, corresponding to a current density of 108 A/cm2 .
CNTs can be used as electron sources in two different types of set-ups, namely single and multiple electron beam devices. One possible application of a single electron beam instrument is an electron microscope that uses an individual CNT or a small CNT bundle as a field emission electron gun to produce a highly coherent electron beam. Conversely, flat panel displays and electron source for X-ray tubes are the most popular example of multiple beam instruments where a continuous or patterned film of CNTs provides a large number of independent electron beams.
density of the film. . Methods such as electrophoresis, printing, self-assembling were developed to fabricate continuous or patterned CNT films for field emission purpose. [50-52]
1.2.3 Other Applications
Carbon materials have been used as electrode materials in fuel cell and batteries for decades. The efficient of fuel cell and batteries depends on the electron transfer rate at the carbon electrode. While structure and morphology of the carbon material determines the electron transfer rate. The porosity and reactivity of CNTs make them ideal replacement for conventional electrode materials. Both MWNTs  and SWNTs [54, 55] are shown to undergo reversible redox reaction with electron donors such as alkali metals resulting in a
significantly reduced electrical resistivity [54, 56] and electronic work function .
Nanometer sized Electronic Devices
Electronic circuits cannot continue to shrink by orders of magnitude and provide corresponding increases in computational power, unless radically different device materials, architectures, and assembly processes are developed. Dramatic recent advances have fueled speculation that nanotubes will be useful for downsizing circuit dimensions.
CNTs can transport terrific amount of electric current without considering doping problem in Si-FETs because the bonds among carbon atoms are much stronger than those in any metal. [61, 62] Recently, several papers have been reported on the CNTs for FETs and CNT-logic applications 
1.3 Conclusions and dissertation overview
And more important lack of bottom up manufacture process that can efficient assemble functional structures and devices using these nano-structured building blocks has been the main hindrance for the applications of CNTs.
1. S. Iijima, Nature 354 (1991) 56
2. L. -C. Qin, X. Zhao, K. Hirahara, Y. Miyamoto, Y. Ando, and S. Iijima, Nature 408 (2000) 50.
3. Thess, R. Lee, P. Nikolaev, H. Dai, P. Petit, J. Robert, C. Xu, Y. H. Lee, S. G. Kim, A. G. Rinzler, D. T. Colbert, G. E. Scuseria, D. Tomanek, J. E. Fischer, R. E. Smalley, Science, 273 (1996) 483.
4. “Image gallery” of a website http://www.pa.msu.edu/cmp/csc/nanotube.html
5. M. S. Dresselhaus, G. Dresselhaus, Ph. Avouris (Eds.) “Carbon Nanotubes: Synthesis, Structure, Properties, and Applications”, Springer-Verlag, Heidelberg, 2001.
6. J. W. G. Wildoer, Nature 391 (1998) 59.
7. W. Moore, Chemistry and Physics of Carbon, 17, P. L. Walker, Jr., P. A. Thrower (Eds.) Dekker, new York (1973)
8. W. Liang, et al., Nature 411, 665 (2001) 9. Stefan Frank et al., Science 280 1744 (1998)
10.Anthony Kendall, Thomas A. Adams II, and Elizabeth Pfaff(1999) 11.P. Chen, X. Wu, J. Lin, K. Tan, Science 285, (1999), 91
12.Liu, Y. Y. Fan, M. Liu, H. T. Cong, H. M. Cheng, M. S. dresselhaus, science 286, (1999), 1127
13.Nutenadel, A. zuttel, D. Chartouni, L. Schlapbach, Solid-State Lett. 2, (1999), 30
14.Chambers, C. Park, R. T. K. Baker, N. m. Rodriguez, J. Phys. Chem. B 102, (1998), 4253 15.J. Hone, M. Whitney, A. Zettle, Synthetic Metals, 103 2498 (1999)
16.S. Berber, Y-K Kwon, and D. Tomànek, Phys. Rev. Lett. 84 (2000) 17.J. F. despres, E. Daguerre, K. Lafdi, Carbon 33, (1995), 87.
19.O. lourie, D. M. Cox, h. D. Wagner, Phys. Rev. Lett. 81, (1998) 1638.
20.J. Muster, M. Burghard, S. Roth, G. S. Dusberg, E. Hernandez, A. Rubio, J. Vac. Sci. Technol. 16, (1998) 2796
21.P. Poncharal, Z. L. Wang, D. Ugarte, W. A. de Heer, Science 283, (1999) 1513 22.R. S. Ruoff, D. C. Lorents, Bull. APS 40, (1995) 173
23.Dekker, Physics Today, (1999) 22.
24.P.M. Ajayan and O.Z. Zhou, Top. Appl. Phys. 80 (2001), 391 25.B. Gao et al., Chem. Phys. Lett., 307, (1999), 153
26.J.S. Sakamoto and B. Dunn, J. Electrochem. Soc. 149 (2002) A39 27.G. Y. Zhang and E.G. Wang, Appl. Phys. Lett. 82, (2003) 1926 28.J. sloan et al., Chem. Commun. (1998) 347
29.C.H. Kiang et. al., J. Phys. Chem. B, 103 (1999) 7449 30.M. Terrones et al., MRS Bull., 43 August (1999)
31.M. Meyyappan, Carbon Nanotubes Science and Applications, CRC press, (2005)
32.V, H, Morris, A. P. Gunning, and A.R. Kirby, Atomic Force Microscopy for Biologists, Imperial college Press, London (1999)
33.Kudo, T. et al. Advances in Resist Technology and Processing XVIII, SPIE Preceedings, 4345, (2001), 179
34.C. V. Nguyen et al. Appl. Phys. Lett., 81, (2002) , 901
35.P. G. Collins, M. s. Arnold, Ph. Avouris, Science, 292 (2001), 706 36.P. G. Collins, et al. Phys. Rev. Lett., 86 (2001), 3128
37.J. Cumings, P. G. Collins, and A. zettl, Nature, 406, (2000), 586 38.C.V. Nguyen et al. J. Phys. Chem. B, 108 (2004), 1816
17 40.T. Arie et al. J. Vac. Sci. Tech. B, 18, (2002), 104 41.N. Yoshida et al. Jpan. J. appl. Phys., 41, (2002) 5013 42.W. Zhu (Ed) “Vacuum Microelectronics” Wiley 2001. 43.Y. Cheng, O. Zhou, C. R. Physique 4 (2003) 1021.
44.W. I. Milne, K. B. K. Teo, G. A. J. Amarantunga, P. Legagneux, L Gangloff, J. –P. Schnell, V. Semet, V. Thien Binh, O. Groening, J. Mater. Chem. 14 (2004) 933.
45.R. H. Fowler, L. W. Nordheim, Proc. R. Soc. (London) A119 (1928) 173.
46.R.Gomer, “Field Emission and Field Ionization”, Harvard University press, Cambridge, MA 1961.
47.Y. Cheng, PhD dissertation, “Carbon nanotube based field emission X-ray sources” 2004.
48.R.Gomer, “Field Emission and Field Ionization”, Harvard University press, Cambridge, MA 1961.
49.D. S. Y. Hsu, Appl. Phys. Lett. 80 (2002) 2988.
50.S. J. Oh, J. Zhang, Y. Cheng, H. Shimoda, and O. Zhou, Appl. Phys. Lett.84, (2004), 3738-3740.
51.S. J. Oh, Y . Cheng, J. Zhang, and H. Shimoda,O. Zhou, Appl. Phys. Lett., 82, (2003), 2521-2523.
52.B. Gao, G.Z. Yue, Q. Qiu, Y. Cheng, H. Shimoda, L. Fleming and O. Zhou, Adv. Mater., 13(11), (2001), 816-819
53.O. Zhou, R. M. Fleming, D.W. Murphy, C. T. Chen, R. C. Haddon, A. P. Ramirez, and S. H. Glarum, Science 263, (1994) 1744–1747.
54.R. S. Lee, H. J. Kim, J. E. Fischer, A. Thess, and R. E. Smalley, Nature (London) 388, (1997) 255.
55.A. M. Rao, P. C. Eklund, S. Bandow, A. Thess, and R. E. Smalley, Nature (London) 388, (1997) 257–259.
57.S. Suzuki, C. Bower, Y. Watanabe, and O. Zhou, Appl. Phys. Lett. 76, (2000) 4007– 4009.
58.W. Liang, et al., Nature 411, 665 (2001)
59.Z. Yao, C. L. Kane, C. Dekker, Phys. Rev. Lett. 84, 2941 (2000) 60.Z. Yao, C. Dekker, Ph. Avouris, Top. Appl. Phys. 80, 147 (2001)
61.R. Martel, T. Schmidt, H. R. Shea, T. Hertel, Ph. Avouris, Appl. Phys. Lett. 73, 2447 (1998).
Chapter 2 Synthesis of Carbon Nanotubes
As it is described in last chapter, CNTs have shown so many intrigue properties that attracted tremendous research efforts to study their potential applications. However, not until a reliable synthesis method, which can provide reasonable amount of CNTs with desirable qualities, is found can those potential applications be truly realized. While CNTs synthesized by different methods may have different characteristics that suits for different applications. Therefore, currently used production methods are studied and a new way to produce CNTs is proposed here and some experimental results will be given.
2.2 Summary of currently used synthesis methods
The first confirmed carbon nanotubes were fabricated using an electric arc discharge between graphite electrodes.  This method had been shown to be successful for the preparation of fullerenes in large quantities.  It was while examing the fullerene products of arc-discharge products that MWNTs were observed. Shortly after, it was discovered that the addition of certain catalyst metals to on of the electrodes produced deposits rich in SWNTs. [3-5]
The basic arc-discharge method involves establishing a DC electric discharge between a pair of graphite electrodes under an inert helium atmosphere (~500 torr). The electrodes are typically water-cooled graphite rods separated by ~1mm with the cathode being of larger diameter than the anode (8-12mm and 6-8mm respectively). A bias of approximately 10-35 V is applied to the electrodes to establish the discharge; currents of ~60-100A and current densities of ~150A/cm2 are typically produced. Achieving a stable discharge plasma is the main factor in generating an environment favorable to nanotube growth. The high temperature arc (> 4000 ºC) leads to sublimation of material from the anode which is transferred to the cathode and surrounding walls of the apparatus.
method is that the process can only last a few minutes before it is terminated by the instability of the DC arc, which is caused by uneven consumption of the anode and build-up of material on the cathode.
2.2.2 Laser Ablation
Like the arc-discharge method, laser-based synthesis of CNTs began as an extension of a process used for fullerene production.  After the first demonstration of using laser ablation to fabricate SWNTs, it has subsequently been used almost exclusively for the synthesis of SWNTs.  Figure 2.1 shows the laser ablation experimental setup in our lab for synthesis SWNTs.
During laser ablation experiment, typically a high power laser beam is used. A target of graphite and transition metal nanoparticles mixture is put in a quartz tube with a quartz window facing the laser beam. The quartz tube is put in a furnace, which is heated up to 900-1200°C (1175 °C in our experiment). The high laser energy densities (50-70J/cm2sec) focused on target surface will evaporate the solid target and form high temperature plumes (3500 to 4000 °C), which is a molten mixture of carbon and catalytic particles. The temperature gradient of the plumes and furnace environment will cause the plumes to expand, and SWNTs will form in the plumes. Then the CNTs along with amorphous carbon and residue catalysts formed in the plum will be carried by the flowing of inert gas (Ar flowing at 400 sccm in our setup) to the quartz tube end, that is wrapped by cooling coils, and deposit there. The laser bean is passed through two scanning prism that will raster scan it across the target surface to get an even consumption of the target.
Theoretically the laser ablation method can provide a continuous production of SWNTs when a big enough target is put into the quartz tube. However after the target is raster-scanned by the laser bean for extended period of time, pits will form on the raster-scanned surface. Therefore, the increased roughness of the target surface will deflect the laser beam, decreased its energy density and slow down the ablation process. For this reason, the laser ablation process usually will be stopped in 12hrs and the target will be taken our and re-polished.
2.2.3 Chemical Vapor Deposition (CVD)
The basic mechanism of CVD involves the pyrolysis of gas-phase carbon-rich molecules (hydrocarbon) in the presence of catalyst at elevated temperatures, and the subsequent conversion of the carbon-fragments (catalytically decomposed from hydrocarbons) into nanotubes. This general procedure had been used to generate carbon fibers and filaments for many years. [18-21] Until 1993 MWNTs were first synthesis by CVD method. 
Figure 2.2 Supported catalysts CVD system, catalyst is deposited on a substrate, which is put into a heated up furnace, hydrocarbon is flowed into the furnace. 
Supported growth is the most widely used CVD-based method of nanotube synthesis. A Preparing the catalyst in advance provides opportunity to define specific patterns for the CNT growth on the substrate. Plasma enhance CVD can also provide control over the growth direction of CNTs. The ability to control the position and direction of growth could have significant benefits, including simple routes to achieving nanotube-based electronic devices. Techniques such as photolithography,  electron beam lithography,  laser etching, [34, 35] and plasma etching have been successfully used to achieve patterned nanotube growth.
Overall, Arc-discharge and laser ablation provide CNTs with relatively higher crytallinity, however at very low yield. CVD methods shows the greatest promise as a true industrial scale process, particularly floating catalyst techniques which, in principle, can be operated in a continuous fashion.
2.3 The method of Laser-CVD
2.3.1 The idea of Laser-CVD
2.3.2 Experiments and Results
The experimental setup is shown in Figure 2.3. A laser ablation chamber described above is used. While respectively 5%, 10% methane is added to the flowing inert gas (Ar). And a pure metal rod (Alfa Aesar: Fe rod 99.99% purity, Ni rod 99.99% purity, Co rod 99.99% purity respectively) is placed in the position of laser ablation target. Iron, Nickel and Cobalt were tried respectively to study their catalytic effect on the CNT growth. While an alloy target with two or more kinds of transition metals may provide a better catalytic effect for CNT growth, it is hard to find such alloy rod commercially. And it’s hard to make a pallet of mixed metal particles that can sustain the high power Laser beam bombardment without being cracked. The furnace is heated up to 800°C instead of 1150°C. A 10Hz pulsed Nd:YAG (Yttrium-Aluminum-Garnet) laser operating at a wavelength of 532 nm is used. The position of the target was determined according to the focal length of the focusing lens so that a focused laser beam with a diameter of 3 mm can fall on the ablated surface. The pulse intensity was 400 mJ/pulse, which, in turn, corresponded to the average intensity density of 5.7 J/cm2⋅pulse. The target surface was raster-scanned with a beam for a uniform
ablation over the entire area.
CVD materials fabricated using different catalyst target and different concentration of hydrocarbon were analyzed by high-resolution transmission electron microscope (HRTEM) and Raman spectroscopy. Results are discussed in the next section.
Figure 2.3 Same setup described in Figure 2.1, a cylinder of methane / Ar mixture is used instead of pure Ar gas and a pure metal target is used.
The Laser-CVD materials collected from the chamber were studied by TEM and Raman spectroscopy. The yield of the Laser-CVD method is comparable with Laser ablation method but is low compared with CVD method, partially due to the low concentration of hydrocarbon is used. However CNTs are produced by using 5% methane and 10% methane. And results show that, higher the concentration of hydrocarbon, higher the yield and higher the purity of the material. While for sake of safety, concentration of hydrocarbon higher then
10% was not attempted. Gas flow rate was increased from 400 sccm to 800 sccm, while there’s no significant increase of the yield. The increase Ar flow may carry the methane and the catalyst particles in the laser plume to the end of quartz tube before their encounter and the pyrolysis of methane in the presence of catalytic particles. Figure 2.4 (b) shows the CNTs made by Laser-CVD method, while pure iron target was used and the hydrocarbon concentration was 10%. Compared with regular laser ablation raw material, the purity of laser-CVD material is still low, however the average bundle size is smaller.
Figure 2.4 TEM images of as synthesized SWNT bundles. (a) SWNTs synthesized by laser ablation method using 0.3% Ni-Co target. (b) SWNTs synthesized by laser-CVD method using iron targe (99.99% purity from Alfar Asear), and 10% methane was added to the flowing gas while flow rate was 400 sccm.
crystallinity and relatively uniform diameters averaged to 1.5 nm. While when iron is used as catalyst, the SWNTs synthesized also have relatively high crystallinity while with a relatively wider diameter distribution from 0.65nm to 2 nm. When cobalt is used as catalyst by itself, the SWNT thus synthesized have corrugated structures as shown in Figure 2.5 (b).
Raman spectroscopy was also used to characterize the SWNTs synthesized by laser-CVD method. The results are shown in Figure 2.6
From the raman spectroscopy shown in Figure 2.6, compared with tw when a particulare wavelengh of Laser was used in this study. Of course, there’s other factors that affects the intensities of the Raman peaks, including density of the Raman samples prepared, bundle sizes, and the electronical structures of the CNTs in the samples. Due the low yield of this method, the CNTs fabricated may not have practical applications, therefore further study was not carrried on.
A summary of the methods currently used to synthesis CNTs are given here. The pros and cons of each method is discussed. Experimental details of synthesis CNTs by laser ablation method were described. The idea of combining laser ablation and CVD method for production of CNTs were porposed. Some experiments were done and the results were discussed.
1. S. Iijima, Nature 356, (1991), 56-58
2. W. Kartschmer, O. L. Lamb, K. Fostiropooulos, D. R. Huffman, Nature 347 (1990), 354-358
3. P.M. Ajayan, S. Iijima, Nature 358, (1992), 23 4. S. Iijima, T. Ichihashi, Nature 363, (1993), 603
5. D.S. Bethund, C.H. Kiang, M.S. de Vries, G. Gorman, R. Savoy, J. Vazquez, R. Beyer, Nature 363, (1993) 605
6. P.M. Ajayan, J.M. Lambert, P. Bernier, L. Barbedette, C. Colliex, Planeix, J.M. Chem. Phys. Lett. 215, (1993), 509–517.
7. C.H. Kiang, W.A. Goddard III, R. Beyers, J.R. Salem, D.S. Bethune, J. Phys. Chem. 98, (1994) 6612–6618.
8. S. Seraphin, D. Zhou, Appl. Phys. Lett. 64, (1994) 2087–2089.
9. J.M. Lambert, P.M. Ahayan, P. Bernier, J.M. Planiex, V. Brotons, B. Coq, J. Castaing, Chem. Phys. Lett. 226, (1994) 364–371.
10.Kiang, C.H.; Goddard III, W.A.; Beyers, R.; Bethune, D.S. Carbon 33, (1995) 903–914. 11.Lambert, J.M.; Ajayan, P.M.; P. Bernier, Synth. Met. 70, (1995) 1475–1476.
12.Journet, C.; Maser, W.K.; Bernier, P.; Loiseau, A.; Lamy de la Chapelle, M.; Lefrant, S.; Deniard, P.; Lee, R.; Fischer, J.E. Nature 388, (1997) 756–758.
13.Y. Ando, S. Iijima, Jpn. J. Appl. Phys. 32 (2000), L1342-L1345
14.H.W. Kroto, J.R. Heath, S.C. O’Brien, R.F. Curl, R.E. Smalley, Nature 318, (1985), 162-163
15.T. Guo, P. nikolaev, A. Thess, D.T. Colbert, R.E. Smalley, Chem. Phys. Lett. 243, (1995) 49-54
16.P.C. eklund, B.K. Pradhan, U.J. Kim, Q. Xiong, J.E. fischer, A.D. friedman, b.C. Holloway, K. Jordan, M.W. Smith, Nano Lett, 2, (2002) 561-566
18.P.L. Walker, J.F. Rakszawski, G.R. Imperial, J. Phys. Chem. 63, (1969), 133-140 19.W.R. Ruston, M. Waezee, J. Hennaut, J. Waty, Carbon 7, (1969), 47-57
20.D. Robertson, Carbon 8, (1970) 365-374
21.T. Baird, J.R. Frayer, B. Grant, Nature 233, (1971) 329-330
22.M.J. Yacaman, M.M. Yoshida, L. Rendon, J.G. santiesteban, Appl. Phys. Lett. 62, (1993) 202-204
23.C.J. Lee, D.W. Kim, T.J. Lee, Y.C. Choi, Y.s. Park, W.S. Kim, Y.H. Lee, W.B. Choi, N.S. Lee, J.M. Kim, Y.G. choi, S.C. Yu, Appl. Phys. Lett. 75, (1999) 1721-1723 24.J. Kong, T.T. Soh, A.M. Cassel, C.F. Quate, H. Dai, Nature 395, (1998) 878-881 25.S. fan, M.G. Chapline, N.r. Franklin, T.W. Tombler, A.M. Cassell, H. Dai, Science 283,
26.D. Xu, G. Guo. L. Gui, Y. Tang, Z. Shi, Z. Jin, Z. Gu, W. Liu, X. Li, G. Zhang, Appl. Phys. Lett. 75, (1999) 481-483
27.S. Huang, A.H.W. Mau, Appl. Phys. Lett. 82 (2003) 796-798
28.K. H. Lee, J. M. Cho, W. Sigmund, Appl. Phys. Lett. 82, (2003) 448-450
29.M.P. siegal, D.L. Overmyer, P.P. Provencio, Appl. Phys. Lett. 80, (2002) 2171-2173 30.C.L. Cheung, A. Kurtz, H. Park, C.M. Lieber, J. Phys. Chem.. B 106, (2002) 2429-2433 31.B.Q. Wei, Z.J. Zhang, P.M. Ajayan, G. Ramanath, Carbon 40, (2002) 47-51
32.C.J. Lee, J. Park, Appl. Phys. Lett. 77, (2000) 3397-3399
33.O.A. Nerushev, S. Dittmar, R.-E. Mrjan, F. rohmund, J. Appl. Phys. 93, (2003) 4185-4190
34.M. Terrones, N. Grober, J. Olivares, J.P. Ahang, H. Terrones, K. Kordatos, W.K. Hsu, J.P. Hare, P.D. Townsend, K. Prassides, a.K. Cheetham, H.W. Kroto, D.R.M. Walton, Nature 388, (1997) 52-55
36.Y. Gao, J. Liu, M. Shi, S.H. Elder, J.W. Virden, Appl. Phys. Lett. 74, (1999) 3642-3644 37.Ch. Emmenegger, P. Mauron, A. Zuttel, Ch. Nutzenadel, A. Schneuwly, R. Gallay, L. 38.Schalapbach, Appl. Surf. Sci. 162, (2000) 452-460
39.X.H. Chen, S.Q. Feng, Y. Ding, J.C. Peng, Z.Z. Thin Solid Films 339, (1999) 6-9
Chapter 3 Processing of Carbon Nanotubes
3.2 Purification and cutting of Carbon Nanotubes
3.2.1 Purification of Carbon Nanotubes
Different methods for purification are used for different types of CNTs. In this dissertation study SWNTs made from laser ablation method in our group are mainly used due to the accessibility of the equipment and the relative reliable quality of these laser ablation materials. While small amount of CNTs were needed in this research, the relatively low yield of laser ablation method did not impose difficulties. As described in chapter 2, in the laser ablation target only 0.3 wt% of catalyst particles were added, which means catalyst particles do not compose major part of the impurities in the raw material. Therefore acid is not needed in the purification process and methods are particularly developed to separate amorphous carbon, graphitic particles and C60 from SWNTs.
The purification schemes that have been developed usually take advantage of the differences in the aspect ratio  and oxidation rate between the nanotubes and the impurities [2,3]. Although the majority of the impurity phases can be eliminated by a combination of filtration and oxidation treatment, these processes also damage the structural integrity of the nanotubes by creating defects on the graphene shells .
A combination of hydrogen peroxide (H2O2) reflux and filtration  is an effective way to
amorphous carbon impurities are preferentially oxidized during the hydrogen peroxide reflux, and their oxidation products are separated from CNTs by filtration. C60 impurities are also
removed by dissolution in carbon disulfide.
Detailed purification process was schematically described in Figure 3.2. 500mg of as produced CNT containing soot was first well dispersed in 400 mL methyl alcohol by bath sonication for 2-3 hours. SWNTs bundles in the raw materials have average length larger then 10 µm, they often tend to entangle and form aggregations in the suspension. This pre-dispersion is to break or soften those entangles, so that a uniform chemical exposure of the material will be achieved. Sometimes, the raw material was also grounded in an electric blender with methyl alcohol to get a uniform dispersion. Then the methyl alcohol is removed by filtering the solution through 2µm pore-size PTFE (poly-tetrafluoro-ethylene) membrane filter (Milipore, Isopore filter). Before the total evaporation of the methanol and re-entanglement of the CNTs, they were placed in 300mL of 20% H2O2 in a round bottom flask.
The flask was placed in a heat mantle to keep the solution at 100°C for the oxidization of amorphous carbon by H2O2. The flask neck was connected to the condenser circulated with
Figure 3.1 Purification of SWNTs produced by laser ablation. (a) A TEM picture of as synthesized SWNTs shows entangled SWNT bundles surrounded by amorphous carbon and catalyst particles. (b) Purified SWNT bundles with purity higher than 90%. (c) The impurities along with some SWNT bundles was filtered through the membrane with the aid of an ultra sonic horn; (d) Illustration of H2O2 reflux system. The SWNT raw material was
oxidized for 8 hours using 20% H2O2 in water. The heat mantle was operated at 100°C. (e)
a sonic wave generating horn was placed inside the solution to keep the CNTs suspended in the medium without sinking down onto the membrane surface to clog the pores and at the same time to separate the oxidized amorphous carbon, isolated catalyst particles and small graphitic particles from the nanotubes. By repeating this process several times until the solution coming down through the filter membrane is almost clear, most oxidation product of amorphous carbon could be removed. During the same process, small amount of isolated catalyst particles are also removed, but some of them attached to the CNTs and covered with graphitic shell were hard to remove without further oxidation using different oxidation chemical reactions.
At the last step, CNTs are suspended in Carbon disulfide and methyl alcohol mixture. Then the suspension is filtered with the aid of the sonic wave generation horn to purify C60 in
the material. Purified CNT film is collected from the surface of the membrane filter and dried in a convection oven overnight. X-ray diffraction (XRD) and TEM measurement using a LEO EM 910 TEM indicate that the purified samples contain ~ 90% SWNT bundles over 10 µm in length and 30-50nm in bundle diameter. (Figure 3.1 (b)) The average SWNT diameter was estimated to be 1.4 nm by x-ray and Raman measurements .
3.2.2 Cutting of Carbon Nanotubes
assembled. Therefore, reducing the CNT bundle length in a controlled way is often desirable. The cutting of CNTs also opens their end tips, allowing the guest species to diffuse into the interior spaces of nanotubes.
The nanotubes can be shortened by ball-milling [8,9], mechanical cutting , and chemical etching [11-13]. Narrower length distribution is always desired in all kinds of applications for short cut CNTs. In this respect, chemical etching is believed to produce better results than ball-milling or mechanical cutting because of the homogeneous nature of a solvent-based process . In chemical etching, purified CNTs are sonicated in concentrated acid so that chemical oxidation can be initiated from the sidewall defects as well as the tips, where the reactivity is higher .
get 2 µm bundle length, 21 hours of sonication is needed, while for 0.5 µm, 30 hours is needed. The etch time and length distribution relations also depend on the quality of the starting material. When cutting CVD grown small diameter MWNTs, much less time is need to get similar length distribution. After the desired etch time, the acid-CNT solution was diluted 10 times with deionized water to prevent further oxidation. The diluted acid mixture was then filtered through a PTFE membrane filter with 0.5µm size pores. Shortened CNTs were collected from the surface of the membrane filter, and dispersed in 300 mL of deionized water to rinse away the residual acid. After repeated filtration and dilution in deionized water, approximately 20 mg (in case of 21 hour etching) of shortened CNTs were collected from the surface of the membrane filter and dried in a convection oven over night. The TEM pictures in Figure 2.4 shows rigid rod-like SWNT bundles of average length 1.5 µm and 0.5 µm, respectively.
3.2.3 Properties of Acid Treated Carbon Nanotubes
Except for the desired length distributions and the rigid-rod morphology, these strong acid oxidized CNTs have other interesting properties.
Open Ended Structure (Accessibility to interior space)
As described in the fist chapter, the porosity and reactivity of the carbon nanotubes (CNTs) make them attractive host materials for storage of neutral species and electron donors . Experimental and theoretical results have shown relatively high storage capacities alkali metals [16,17], suggesting potential applications for fuel cells and rechargeable batteries. One of the key parameters that determine the applicability of the CNTs for energy storage is the amount of materials/charges that can be stored per unit weight. This is determined in part by the accessibility of the interior spaces of the CNTs for diffusion. Experiments of lithium intercalation have shown that the lithium/carbon ratio increases from LiC6 to LiC3 after the CNTs are etched in strong acid . Similar results have also
been observed for other guest species such as methane  and C60 fullerenes. The large
increase is attributed to diffusion of additional Li ions into the interior spaces of the SWNTs through the open ends and possibly the defective sides on the sidewalls. Opening of the tube ends in oxidizing environment have been reported in several studies. The effects of exposing CNTs to different oxidizing agents from mild oxidizing gas [20-22] to strong acids [23,24] have been investigated.
bundles is shown in figure 3.4 (a). While a HRTEM image of the bundle ends is shown in Figure 3.4 (b). The outer surfaces of the bundles were coated with amorphous carbon, which was presumably produced by the etching process. The ends of the SWNT bundles have a tapered morphology suggesting that the etching process starts both laterally and longitudinally. The detailed structure of the individual SWNTs was not resolved because the abundance of the amorphous carbon.
Figure 3.4: a) Low resolution TEM image of acid treated SWNT bundles before annealing to show the average bundle length is about 1µm, the scale bar is 0.5µm; b) High resolution TEM image of acid treated SWNT bundles, showing blurred edge of the bundles, indicating that they are wrapped with amorphous carbon after the acid treatment. The tapered ends also suggest that etching process happens both lateral and longitudinal.
The same batch of sample was vacuum annealed at 400˚C for 10hr under 510-6 torr base
pressure. Then it was studied by HRTEM. HRTEM images of 20 individual tubes were taken from the sample. The results show that the tips of overwhelming majority of the SWNTs were opened by the oxidation process and remained open after annealing (Figure 3.5). This is consistent with the prior Li intercalation  and gas uptake  experiments, which showed a large increase of the storage capacity after the SWNTs were etched and annealed at 500 ˚C
0.5µm 50 nm
in vacuum . The surfaces of these SWNT bundles have much less amorphous carbon and the bundles have better crystallinity than those before annealing, as shown by the TEM images.
Figure 3.5 HRTEM images of individual SWNTs after oxidation and vacuum annealing at 400 oC for 10hrs. The results show that the ends of the SWNTs stayed open after the 400 oC annealing. (The scale bar is the same for all 4 images)
The reduced aspect ratio of the shortened SWNT bundles was 50-100 depending on the
Figure 3.6 Raman spectroscopy data from chemically oxidized SWNTs indicates unchanged frequency of the characteristic RBM mode.
3.3 Regraphitization of the Carbon Nanotubes by High Temperature Annealing
The regraphitization of carbon nanotubes by high temperature annealing was studied here to gain further control over the structure of the processed carbon nanotubes. Although the regraphitization of CNTs has been the subject of several theoretical investigations [25, 26] there is no report on re-graphitization of the defects in bulk CNT materials.
expected temperature. The observation is confirmed in bulk samples by proton NMR measurements of the amount of ethane uptake at different processing stages. The re-graphitized SWNT tips have a variety of morphologies that are different from the ideal hemispherical structure. The results demonstrate the structure of the SWNTs in bulk quantities can be modified in a controlled fashion to optimize their materials properties.
3.3.1 HRTEM Analysis
After TEM observations the same batch of acid treated SWNTs discussed in last section was annealed at 800˚C for 1hr at 510-6 torr. Figure 3.7 shows the typical TEM micrographs taken from the same sample after annealing at 800˚C. The tips of 19 out of the 20 individual SWNTs observed were closed and/or covered with some disordered structures. The closed tube ends were found to have various morphologies instead of the perfect hemispherical structure. For example flat and irregular cap structures were often observed as shown in Figure 3.8 (i). Some of the tips were covered with disordered structures as shown in Figure 3.8 (e)-(h). The exact nature of these structures is unclear. They are possibly chemical groups attached to the nanotube tips or the amorphous carbon formed either during the oxidation process or by contamination formed during TEM observation. Out of the 20 clear images of the individual SWNT tips taken, only one showed an open-ended structure.
Figure 3.7 HR-TEM images of individual SWNTs after oxidation and annealing first at 400oC for 10hrs then at 800 oC for 1hr. (The figures share the same scale bar.)
3.3.2 Gas Absorption Experiment and Results
Since TEM studies are intrinsically limited by the fact that the number of nanotubes observed is a very small fraction of the total sample, NMR technique was utilized to investigate the effect of oxidation and vacuum annealing on the bulk SWNT samples. The hypothesis of this approach is that gas adsorption capacity is correlated to the accessibility of the interior space of the nanotubes which can be modified by oxidation and annealing. This has been confirmed by our previous studies that showed the amount of methane adsorption increased significantly after the SWNTs were etched by oxidation .
The SWNT sample was put into a quartz NMR tube connected to a vacuum pump and an ethane cylinder. The experiment was performed at room temperature in the pressure range of 0-0.6MPa of C2H6. Data were analyzed using the method published in reference . In
brief, since the intensity of the NMR spectrum is proportional to the numbers of proton spins in the observed volume, it changes with the gas pressure and the adsorption capability of the SWNT sample. The NMR spectrum at certain pressure is composed of a sharp peak and a broad peak. The sharp peak, which is only proportional to the gas pressure, is attributed to gas molecules in the region of the NMR sample tube unoccupied by SWNTs. The intensity of the broad peak, whose dependence on the gas pressure is plotted in Figure 3.8, shows characteristic behaviors of adsorption.
0.0 0.1 0.2 0.3 0.4 0.5 0.6 0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5
C2H6 adsorption (mmol/g)
C2H6 pressure: Mpa
C2H6 adsorption in cut SWNT C2H6 adsorption in annealed SWNT
Figure 3.8 Pressure dependence of the intensities of the broad peaks of the 1H NMR
The amount of ethane uptake was measured for the etched sample and the same sample after 800oC annealing obtained from the in-situ proton NMR experiment. As shown in Fig. 4, the amount of C2H6 stored in the etched SWNTs reached the level of ~3.5mmol of C2H6 per
gram of SWNTs at 0.6MPa which is to be compared with the 0.4 mmol/gram in pristine SWNTs that we reported previously . The adsorption rate after annealing at 800oC dropped significantly to became comparable to that of the as purified pristine SWNTs (with close-end structure). At 0.6MPa, the amount of C2H6 uptake reduced to 0.8mmol/gram.The
NMR result also showed that the amount of proton-containing chemical groups such as carboxyl or/and hydroxyl group were reduced significantly after the high temperature annealing.
The NMR result is consistent with the conclusion from the TEM study that the tips of most of the SWNTs were closed after annealing at 800oC. This re-graphitization temperature is lower than the temperature predicted by theoretical calculations [13, 25]. First-principles molecular dynamics simulations show that open-end SWNT closes spontaneously into graphitic dome with no residual dangling bonds at 2000K-3000K . A recent electron field emission study showed that the SWNT tip can be opened under high emission current and closed again when the current is decreased at an estimated tip temperature of 1600K induced by the emission current.
sample heat treated at 400˚C has also indicated the migration of amorphous carbon along the tube wall. The forming of a flat cap structure was simulated using the Cerius2 software by introducing pentagons and atomic carbon to an open end (10, 10) SWNT. After relaxation was allowed this structure was found to be metastable, though energetically less stable than perfect hemispherical caps.
1. K. B. Shelimov, R. O. esenaliev, A. G. Rinzler, C. B. Huffman, R. E. Smalley, Chem. Phys. Lett. 282 (1998) 429.
2. T. W. Ebbesen, P. M. Ajayan, H. Hiura, K. Tanigaki, Nature 367 (1994) 519.
3. K. Tohji, T. Goto, H. Takahashi, Y. Shinoda, N. Shimizu, B. Jeyadevan, I. Matsuoka, Y. Saito, A. Kasuya, T. Oshuna, K. Hiraga, Y. Nishina, Nature 383 (1996) 679.
4. M. Monthioux, B. W. Smith, B. Burteaux, A. Claye, J. E. Fischer, D. E. Luzzi, Carbon 39 (2001) 1251.
5. O. Zhou, B. Gao, C. Bower, L. Fleming, H. Shimoda, Mol. Cryst. Liq. Cryst. 340 (2000) 541.
6. Soojin Oh’s Dissertation
7. X.P. Tang, A. Kleinhammes, H. Shimoda, L. Fleming, C. Bower, S. Sinha, O. Zhou, and Y. Wu.. Science 228 (2000) 492.
8. B. Gao, C. Bower, J. Lorentze, L. Fleming, A. Kleinhammes, X. P. Tang, L. E. McNeil, Y. Wu, and O. Zhou, Chem. Phys. Lett. 327 (2000) 69.
9. N. Pierard, A. Fonseca, Z. Konya, I. Willems, G. van Tendeloo, J. B. Nagy, Chem. Phys. Lett. 335 (2001) 1
10.I. Stepanek, G. Maurin, P. Bernier, J. Gavillet, A. Loiseau, R. Edwards, O. Jaschinski, Chem. Phys. Lett. 331 (2000) 125
11.H. Shimoda, B. Gao, X. P. Tang, A. Kleinhammes, L. Fleming, Y. Wu, and O. Zhou, Phys. Rev. Lett. 88 (2002) 015502
12.P. M. Ajayan, T. W. Ebbesen, T. Ishihashi, S. Iijima, K. Tanigaki, H. Hiura, Nature 362 (1993) 522.
13.J. Liu, A. G. Rinzler, H. Dai, J. Hafner, A. R. Bradley, P. Boul, A. Lu, T. Iverson, A. K. Shelimov, C. B. Huffman, F. Rodriguez-Macias, Y. Shon, R. Lee, D. T. Colbert, R. E. Smalley, Science 280 (1998) 1253.
16.R.S. Lee, H.J. Kim, J.E. Fischer, A. Thess, and R.E. Smalley.Nature, 388: (1997) 255-257.
17.H. Shimoda, B. Gao, X.P. Tang, A. Kleinhammes, L. Fleming, Y. Wu, and O. Zhou Phys. Rev. Lett.,. 88(1) (2002) 015502.
18.A. Kleinhammes, S.H. Mao, X.J. Yang, X.P. Tang, H. Shimoda, J.P. Lu, O. Zhou, and Y. Wu.Phys. Rev. B, 68(7), (2003) 075418-1-6.
19.Smith B.W. and D.E. Luzzi.Chem. Phys, Lett, 321 (2000) 169-174.
20.S. C. Tsang, P. J. F. Harris, M.L. H. Green. Nature 362, (1993) 520
21.P. M. Ajayan, T. W. Ebbesen, T. Ichihashi, S. Iijima, K. Tanigaki, H. Hiura, Nature 362, (1993) 522
22.Hiura, H; Ebbesen, T (1997). U.S. Patent No.5,698,175. Washington, DC: U.S. Patent and Trademark Office.
23.J. Sloan, J. Hammer, M. Z. Sibley, M. L.H. Green, Chem. Commun., (1998) 347 24.J.C. Charlier; X. Blasé; A. De Vita; R. Car; Applied Physics A. 68 (1999) 267 25.K. A. Dean; B. R. Chalamala J. Vacuum Society Techonlogy B 21(2), (2003) 868
26.H. Geng, X. B. Zhang, S. H. Mao, A. Kleinhammes , H. Shimoda ,Y. Wu, O. Zhou
Chapter 4 Manipulation and Assembly of CNTs by
In the previous chapters, it is described clearly that carbon nanotubes (CNTs) have become an important class of materials for both fundamental studies and technological applications . Considerable progress has been made recently in understanding the formation mechanism and in developing synthesis routes for fabrication of homogeneous CNTs with controlled structure and morphology and in further process procedure to tune their properties. However eventual utilization of these novel materials in the wide range of applications such as sensors, electron field emitters and microelectronics, requires new processes for controlled assembly and integration, which is current lacking.
to separate metallic SWNTs from semiconducting SWNTs. Here a close study on the possibilities of assembly CNTs into functional structures by dielectrophoresis is carried on. Effects of some experimental conditions including the viscosity, ionic conductivity of the medium, and the frequency and amplitude of the AC field are systematically studied. The feasibility of fabricating CNT structures connecting differently patterned electrodes were researched; And CNT fibrils attached to sharp tips, which have versatile applications, were fabricated.
4.2.1 Dielectrophoretic Force
Figure 4.1 Illustration of Dielectrophoresis. 
strength is different on the two sides of the particle, a net force acts on the particle. This is termed as dielectrophoresis. (Figure 4.1)
The dielectrophoretic force F(t) on a particle is given by the following general expression :
where m (t) is the polarizability of the particle and E (t) is the electrical field. A CNT or bundle can be considered as a rod shaped particle with very large aspect ratio. When a rod shaped particle is placed in the electrical field, it will experience a torque, which tends to align one of the particle’s axes with the field. The rod will align so that all components of torque are zero. The magnitude and orientation of the torque depend on the frequency of the applied field and the properties of the particle and the medium. The orientation of a rod shaped particle can be controlled by the conductivity of the medium and the frequency of the applied field3. The dielectrophoretic force on a rod whose major axis is parallel to the electric field is given by equation (2).
Where a,b,c are the dimensions and εp* is the permittivity of the rod. εm* is the permittivity of
the medium. ε* is given by equation (3)
Where σ is conductivity, and ϖ is the frequency of the AC field. From these equations,
permittivity, conductivity of the suspending medium and the frequency of AC field are shown to be critical parameters. And the properties of CNTs are not variables in our experiments when certain types of CNTs are used.
From equation (2), when the permittivity of the particle is larger than that of the medium, dielectrophoretic force is positive and the particles will move to areas with high electrical field concentration. While when the permittivity of the particle is smaller than that of medium, negative dielectrophoresis will happen, where particles move to areas with low field concentration. This phenomenon is widely used in biology to separate live and dead cells, because they have different ion concentrations in their plasma. And it can potentially be used to separate metallic and semiconducting SWNTs when they are exfoliated into individual tubes by the aid of surfactants.  Experiments with successful results were reported,  however there are still doubts on the interpretation of the results. [15-17]
59 4.2.2 Torque and Alignment
Particles possessing any kind of polarization anisotropy will experience a torque that tends to align the particle with some preferred axis parallel to the applied electric field.  A freely suspended insulating ellipsoid always tends to align itself with its longest axis parallel to the imposed field. This alignment hehavior is completely independent of the relative magnitudes of its permittivity or the permittivity of the suspending medium. However when CNT bundles suspended in DI water are subjected to AC field, as conducting particles they may exhibit a frequency dependent orientational effect called an orientational spectrum. There always will be a pair of turnover points, where the particle changes its orientation. And if this pair of points do exist, parallel orientation (where long axis parallels the direction of the electric field) is always favored at the lowest and highest frequencies; The particle first changes from parallel to perpendicular orientation and then back to parallel as frequency is increased. 
Figure 4.2 Illustration of an elongated particle suspended in AC field. 
Figure 4.2 shows a rod shaped particle put into an AC field with angle θ between its long
(with no conduction or dielectric conduction), the time averaged alignment torque with respect to z-axis is given by equation (4) :
3 Te z
Where a, b are the dimensions of the particle, E0 is the amplitude of the applied field and Cs
is the nondimensional torque and will be referred to as torque constant. And Cs can be
approximated in equation (5) when the particle has very large aspect ratio:
)(5) From equation (5), it is clear that a negative value of Cs will ensure that the parallel
orientation be a stable orientation. Otherwise a positive value of Cs ensures that perpendicular
orientation be the stable orientation.
To solve the rotation equation by balancing the alignment torque and a resistant force caused by the viscosity of the medium, the order of magnitude of the rod’s responding time to the alignment torque is given by equation (6).
Where η is the viscosity of the suspending medium and Ks is a shape factor and can be
approximated in equation (7) when the particle has large aspect ratio:
the pitch time of electrical field, otherwise the particle will oscillate about the mean orientation. That means tR is much larger than 1/ω and this condition can be approximated in
expression (8) when the particle has large aspect ratio :
There’s a threshold value of the AC frequency, only when AC frequency is larger than the threshold value, expression (8) is valid, and then alignment may happen. This threshold value can be lowered by increasing the viscosity of the medium. This is a very simple model, which assumes CNTs as lossless particles, as it is used in reference . This model is explained here to shine some light on the experimental results that will be discussed later.
4.3 Experimental Setup